1.55k likes | 2.18k Vues
Extraction Metallurgy. Part 2: Case studies. Dr. C.B. Perry (C306). http://www.gh.wits.ac.za/chemnotes. Chem 3033. Extraction Metallurgy. Part 2: Case studies. Copper – Pyrometallurgy route and environmental concerns. The hydrometallurgical alternative.
E N D
Extraction Metallurgy Part 2: Case studies Dr. C.B. Perry (C306) http://www.gh.wits.ac.za/chemnotes Chem 3033
Extraction Metallurgy Part 2: Case studies • Copper – Pyrometallurgy route and environmental concerns. The hydrometallurgical alternative. • Hydrometallurgical processes – ion exchange processes, solvent extraction, and bacterial leaching. • Iron – Pyrometallurgy and the blast furnace. • Silicon – The electric arc furnace. Purification by the Czochralski process. • Aluminium – Electrolytic reduction. • The siderophiles – The extraction of Au and the Pt group metals and their purification.
Pyrometallurgy of copper Reminder: Pyrometallurgy is the use of heat to reduce the mineral to the free metal, and usually involves 4 main steps: • Calcination:thermal decomposition of the ore with associated elimination of a volatile product. • Roasting: a metallurgical treatment involving gas- solids reactions at elevated temperatures. • Smelting: a melting process which separates the chemical reaction products into 2 or more layers. • Refining: treatment of a crude metal product to improve its purity.
Pyrometallurgy of copper Cu ore usually associated with sulphide minerals. Most common source of Cu ore is the mineral chalcopyrite (CuFeS2), which accounts for ± 50% of Cu production. Other important ores include: chalcocite [Cu2S], malachite[CuCO3 • Cu(OH)2], azurite [2CuCO3• Cu(OH)2], bornite (3Cu2S • Fe2S3), covellite (CuS).
Pyrometallurgy of copper The following steps are involved in Cu extraction: • Concentration • Roasting • Smelting • Conversion • Refining
Pyrometallurgy of copper 1. Concentration Finely crushed ore concentrated by the froth-flotation process: • Ground ore mixed with xanthates (salts & esters of xanthic acid), dithiophosphates, or thionocarbamates. These make the ore surface hydrophobic. • Ore then introduced into a water bath where air is bubbled through the suspension. • Finely divided hydrophobic ore particles latch on to the air bubbles and travel to the surface where a froth is formed.
Pyrometallurgy of copper 1. Concentration (cont.) • The froth containing the Cu ore is skimmed off and reprocessed. • The remaining material (sand particles & other impurities) sink to the bottom & is discarded or reprocessed to extract other elements.
Pyrometallurgy of copper 1. Concentration (cont.) Froth-flotation
Pyrometallurgy of copper 2. Roasting • Involves partial oxidation of the sulphide mineral with air at between 500C and 700C. • For chalcopyrite, the main reactions are: • CuFeS2(s) + 4O2(g) → CuSO4(s) + FeSO4(s) • 4CuFeS2(s) + 13O2(g) → 4CuO(s) + 2Fe2O3(s) + 8SO2(g) • Reactions are exothermic, roasting is an autogenous process requiring little or no additional fuel. • NB, not all the sulphides are oxidised, only around 1/3. Rest remain as sulphide minerals. • The gases produced contain around 5 – 15% SO2, which is used for sulphuric acid production.
Pyrometallurgy of copper 2. Roasting (cont.) Objectives of roasting: 1) Remove part of the sulphur. 2) Convert iron sulphides into iron oxide and iron sulphate to facilitate removal during smelting. 3) To pre-heat the concentrate to reduce amount of energy needed by the smelter.
Pyrometallurgy of copper 3. Smelting • Smelting consists of melting the roasted concentrate to form 2 molten phases: • 1) a sulphide “matte”, which contains the iron-copper sulphide mixture. • 2) an oxide slag, which is insoluble in the matte, and contains iron oxides, silicates, and other impurities. • Smelting is carried out at around 1200C, usually with a silica flux to make the slag more fluid. • The matte layer sinks to the bottom, and the slag layer floats on top of the matte & is tapped off & disposed of.
Pyrometallurgy of copper 3. Smelting (cont.) • The main reaction is the reduction of copper oxides (formed during roasting) back into copper sulphide to ensure that they migrate into the matte phase: • FeS(l) + 6CuO(l) → 3Cu2O(l) + FeO(l) + SO2(g) • FeS(l) + Cu2O(l) → FeO(l) + Cu2S(l) • Cu2S(l) + FeS(l) → Cu2S•FeS(l) (matte)
Pyrometallurgy of copper 4. Conversion • After smelting, matte contains from between 30 to 80% Cu in the form of copper sulphide. • The sulphur is removed by selective oxidation of the matte with O2 to produce SO2 from S, but leave Cu metal. • Converting is carried out in two stages: 1) an iron removal stage, and 2) a copper-making stage.
Pyrometallurgy of copper 4. Conversion (cont.) Iron removal • A silica flux is added to keep the slag (see below) molten. • Air is blown into the converter to oxidize the iron sulphide according to the following reaction: • 2Cu2S•FeS(l) + 3O2(g) + SiO2(l) → 2FeO•SiO2(l) + 2SO2(g) + Cu2S(l) • The oxidized Fe and Si form a slag (insoluble in matte) that is skimmed off & disposed off.
Pyrometallurgy of copper 4. Conversion (cont.) Copper making • The sulphur in the Cu2S can now be oxidized to leave behind metallic copper according to the following reaction: • Cu2S(l) + O2(g) → 2Cu(l) + SO2(g) • The end product is around 98.5% pure & is known as blister copper because of the broken surface created by the escape of SO2 gas.
Pyrometallurgy of copper 5. Refining • The copper is refined by electrolysis. • The anodes (cast from blister copper) are placed into an aqueous CuSO4/H2SO4 solution. • Thin sheets of highly pure Cu serve as the cathodes. • Application of a suitable voltage causes oxidation of Cu metal at the anode. • Cu2+ ions migrate through the electrolyte to the cathode, where Cu metal plates out.
Pyrometallurgy of copper 5. Refining (cont.) • Metallic impurities more active then Cu are oxidized at the anode, but don’t plate out at the cathode. • Less active metals are not oxidized at the anode, but collect at the bottom of the cell as a sludge. • The redox reactions are: • Cu(s) Cu2+(aq) 2e- • Cu2+(aq) + 2e- Cu(s) Ered = -0.83V
Pyrometallurgy of copper 5. Refining (cont.)
Pyrometallurgy of copper Environmental impact • Large amount of gases produced present air pollution problems, in particular SO2 gas acid rain. • Dust produced contains heavy metals such as mercury, lead, cadmium, zinc health problems. • Waste water contaminated with: • Insoluble substances, mostly waste sludge (finely ground rock). • Soluble substances (heavy metals, sulphates). • Chemicals from flotation process.
Hydrometallurgy of copper Advantages • Much more environmentally friendly than pyrometallurgy. • Compared to pyrometallurgy, only a fraction of the gases liberated into the atmosphere. • Emissions of solid particles comparatively non-existent. Disadvantages • Large amount of water used, greater potential for contamination. • Waste waters contain soluble metal compounds, chelating compounds & organic solvents.
Hydrometallurgy of copper The following steps are involved: • Ore preparation • Leaching • Solution purification • Metal recovery
Hydrometallurgy of copper 1. Ore preparation • Ore undergoes some degree of comminution (crushing & pulverisation) to expose the Cu oxides & sulphides to leaching solution.
Hydrometallurgy of copper 1. Ore preparation (cont.) • Amount of comminution depends on quality of ore: • Higher grade ore – more comminution. • Lower grade ore – less comminution. • (Why??) • If possible, ore is pre-concentrated; reject ore that contains very little Cu.
Hydrometallurgy of copper 2. Leaching Definition : The dissolution of a mineral in a solvent, while leaving the gangue (rock or mineral matter of no value) behind as undissolved solids. • Cu is normally leached by one of three methods: • Dump leaching • (b) Heap leaching • (c) Bacterial leaching
Hydrometallurgy of copper 2. Leaching (cont.) (a) Dump leaching • Leaching solution trickled over a dump. • Runoff solution collected & the Cu recovered from it. • A slow process that takes months or years to complete. • Typically only around 60% of the Cu in the dump is recovered.
Hydrometallurgy of copper 2. Leaching (cont.) (b) Heap leaching • Similar to dump leaching except ore not simply dumped on a hillside, but is crushed to gravel size & piled onto an artificial pad. • After leaching (6 months to 1 year) gangue is removed from pad, disposed of & replaced with fresh ore.
Hydrometallurgy of copper 2. Leaching (cont.) Leaching reactions Nature of ore determines if leaching is non-oxidative or oxidative. Non-oxidative leaching: No change in oxidation state. e.g. (1) dissolution of copper sulphate by water: CuSO4(s) + H2O(l) Cu2+(aq) + SO42-(aq) (2) dissolution of alkaline materials by acid: Cu2(OH)2•CO3(s) + 2H2SO4(aq) 2CuSO4(aq) + CO2(g) + 3H2O(l)
Hydrometallurgy of copper 2. Leaching (cont.) Oxidative leaching: Many ores only soluble once oxidised. e.g. covellite (CuS) much more soluble if oxidised to CuSO4 CuS(s) + O2(g) CuSO4(aq) CLASS EXERCISE : work out which species is oxidised, and which is reduced, and write out the balanced half reactions for each. SOLUTION: CuS Cu = +2, S = -2 O2 O = 0 CuSO4 Cu = +2, O4 = -8, S = +6 S-2 S+6 + 8e- (oxidation) 2O2 + 8e- 4O2- (reduction)
Hydrometallurgy of copper 2. Leaching (cont.) (c) Bacterial leaching • Several bacteria, especially Thiobacilli, are able to solubilise metal minerals by oxidising ferrous to ferric iron, as well as elemental sulphur, sulphide, and other sulphur compounds to sulphate or sulphuric acid. • 20 to 25% of copper produced in the USA, and 5% of the worlds copper is obtained by bacterial leaching. • Very slow process; takes years for good recovery • But low investment and operating costs.
Hydrometallurgy of copper 2. Leaching (cont.) (c) Bacterial leaching Thiobacilli • Are acidotolerant; some grow at pH’s as low as 0.5 • Are tolerant against heavy metal toxicity. • Are chemolithoautotrophs (C source is CO2 & energy derived from chemical transformation of inorganic matter).
Hydrometallurgy of copper 2. Leaching (cont.) (c) Bacterial leaching Mechanisms Generalised reaction : M(II)S + 2O2 M2+ + SO42- • Two mechanisms: (a) indirect mechanism involving the ferric-ferrous cycle, and (b) direct mechanism involving physical contact of the organism with the sulphide mineral.
Hydrometallurgy of copper 2. Leaching (cont.) (c) Bacterial leaching Mechanisms: Indirect First step: ferrous sulphate is converted into ferric sulphate by the action of Acidithiobacillus ferrooxidans: 4FeSO4 + O2 + 2H2SO4 2Fe2(SO4)3 + 2H2O CLASS EXERCISE : work out which is ferric- and which is ferrous sulphate, and write out the balanced half reactions for each. FeSO4– SO42- Fe2+ (ferrous) 2Fe2(SO4)3 – 3 × SO42- = -6, but 2 × Fe Fe3+ (ferric)
Hydrometallurgy of copper 2. Leaching (cont.) (c) Bacterial leaching Mechanisms: Indirect 2Fe2+ 2Fe3+ + 2e- (oxidation) O2 + 2e- 2O2- (reduction) • Ferric sulphate is a strong oxidising agent capable of dissolving a range of sulphide minerals. • In the case of chalcopyrite: CuFeS2 + 2Fe2(SO4)3 CuSO4 + 5FeSO4 + 2S
Hydrometallurgy of copper 2. Leaching (cont.) (c) Bacterial leaching Mechanisms: Indirect • The elemental S produced by the indirect method can be converted to H2SO4 by Acidithiobacillus ferrooxidans: • The H2SO4 helps maintain the pH at levels favourable for bacterial growth.
Hydrometallurgy of copper 2. Leaching (cont.) (c) Bacterial leaching Mechanisms: Direct • Bacteria actually adheres to the mineral surface prior to enzymatic attack. • The mineral is oxidised with oxygen to sulphate and metal cations without any detectable intermediate occurring. • In the case of covellite: CuS + 2O2 CuSO4
Hydrometallurgy of copper 3. Solution Purification • Leaching reactions not perfectly selective other elements in solution as well, not just Cu. These need to be removed. • After leaching, Cu in solution can be very dilute. need a way to concentrate it. • Both of these are generally done using ion exchange processes, the two most common being ion exchange chromatography, and solvent extraction.
Hydrometallurgy of copper 3. Solution Purification Ion exchange chromatography • DEFINITION: a solution containing a mixture of metal ions is contacted with a resin that is insoluble in the metal-ion solution. • Ion-exchange resin consists of an inert solid phase to which labile functional groups are chemically bonded. • Functional groups can either be acidic (H+) or basic (OH–) groups that exchange with cations (M+) or anions (M–), respectively. • The ion-exchange process is reversible.
Hydrometallurgy of copper 3. Solution Purification Ion exchange chromatography • Carboxyl groups exchanges the ion it currently holds (H+) for a Cu2+ ion. • The Cu2+ is later released by contacting it with a stripping solution (very high H+ conc.).
Hydrometallurgy of copper 3. Solution Purification: Solvent extraction • DEFINITION: a method to separate compounds based on their relative solubilities in 2 different immiscible liquids. • In industry, this is usually set up as a continuous process
Hydrometallurgy of copper 3. Solution Purification: Solvent extraction
Hydrometallurgy of copper 3. Solution Purification: Solvent extraction • Organic + aqueous stream pumped into a mixer. • Organic (containing an extractant) and aqueous components mix, and ion transfer occurs between them. • Once ion transfer is complete (equilibrium), mixture is allowed to separate. • Aqueous solution is removed & the organic phase (containing the Cu2+) is mixed with an aqueous stripping solution. • Cu2+ moves back into the aqueous phase, and the two phases are again allowed to separate. • The aqueous phase (containing the Cu2+) is removed & the organic phase is recycled back into the first mixer.
Hydrometallurgy of copper 3. Solution Purification: Solvent extraction Extractants • The most successful extractants for copper are of the ortho-hydroxyoxime type: R = alkyl ,phenyl, or H R1 = alkyl • Function by means of a pH-dependent cation-exchange mechanism: Cu2+ + 2HA CuA2 + 2H+ (where H in HA denotes the replaceable, phenolic proton)
Hydrometallurgy of copper 3. Solution Purification: Solvent extraction Extractants • At low pH (1.5 – 2.0) the ortho-hydroxyoxime extractant complexes the Cu. • During back-extraction (stripping stage) the pH is lowered further, releasing the Cu, and regenerating the hydroxyoxime for recycle to the extraction stage. • Aqueous feeds (leach solution) typically contain more iron per litre than copper. For commercial success, the extractant must have a greater selectivity for Cu than Fe.
Hydrometallurgy of copper 3. Solution Purification: Solvent extraction Extractants • Cu2+ forms square-planar complexes with hydroxyoxime: • H-bonding between the oximic H and the phenolic O affords this 2:1 complex unusual stability. • The formation constant (K2) for the 2:1 complex is much greater than for the 1:1 complex.
Hydrometallurgy of copper 3. Solution Purification: Solvent extraction Extractants • The tris(salicylaldoximato)iron(III) complex is octahedral, and no extended planar ring structure is possible between the 3 oxime ligands. • stability of Fe(III) complex is less than Cu(II) complex, which allows the extraction of Cu to be carried out at lower pH than what is required for efficient Fe extraction.
Hydrometallurgy of copper 4. Metal Recovery: • At this point, the metal needs to be recovered from solution in the solid form. • This is either achieved chemically, or electrochemically.
Hydrometallurgy of copper 4. Metal Recovery: Chemical recovery • Dissolved copper will plate out on an iron surface according to the following reaction: Cu2+(aq) + Fe(s) Fe2+(aq) + Cu(s) Why?? Reduction half-reactions: Cu2+(aq) + 2e– Cu(s) Ered = +0.34 V Fe2+(aq) + 2e– Fe(s) Ered = -0.44 V • Ered for the Cu2+ half-reaction is more positive than for the Fe2+ half reaction which leads to Cu being reduced and Fe oxidised.
Hydrometallurgy of copper 4. Metal Recovery: Chemical recovery • Solutions containing dissolved copper are thus run through a bed of shredded scrap iron, resulting in the copper ions being plated out as solid Cu on the iron surface. • For the process to be efficient, the surface of the scrap iron must be large.
Hydrometallurgy of copper 4. Metal Recovery: Electrochemical recovery Electrowinning • An electrochemical process for precipitating metals from solution.
Hydrometallurgy of copper 4. Metal Recovery: Electrochemical recovery Electrowinning • A current is passed from an inert anode through a liquid leach solution containing the metal so that the metal is extracted as it is deposited onto the cathode. • The anode is made out of a material that will not easily oxidise or dissolve, such as lead or titanium.